Equivalent CO2 Emission and Cost Analysis of Green Self-Compacting Rubberized Concrete

Global warming and climate changes are the major environmental challenges globally. With CO2 emission being one of the main greenhouse gases emitted to the environment, and cement and concrete production amounting to about 10% of the global CO2 emission, there is a need for the construction industry to utilize an environmentally sustainable material as an alternative to cement. This study analyzed the cost, CO2 emission and strength properties of green self-compacting concrete (SCC) ternary blend containing fly ash, calcium carbide residue (CCR), and crumb rubber (CR) as a replacement material by volume of cement, cementitious material, and fine aggregate, respectively. Cement was replaced with fly ash at 0 and 40% by volume. CCR was used as a replacement at 5 and 10% by volume of cementitious materials, CR replaced fine aggregate in proportions of 10 and 20% by volume. The result indicated that the mix with 0% fly ash and 20% CR replacement of fine aggregate was the most expensive and had the highest CO2 emission. However, the mix with 10% CR, 40% fly ash, and 10% CCR had the lowest CO2 emission and was therefore the greenest SCC mix. The 28-day maximum compressive strength of 45 MPa was achieved in a mix with 0% CR, 0% fly ash, and 10% CCR, while the utmost 28-day splitting tensile strength of 4.1 MPa was achieved with a mix with 10% CR, 0% fly ash, and 5% CCR, and the highest flexural strength at 28 days was 6.7 MPa and was also obtained in a mix with 0% CR, 0% fly ash, and 5% CCR. In conclusion, a green SCC can be produced by substituting 40% cement with fly ash, 10% fine aggregate with CR, and 10% CCR as a replacement by volume of cementitious material, which is highly affordable and has an acceptable strength as recommended for conventional SCC.


Introduction
Climate change has emerged as a major environmental concern. Environmental sustainability is the major challenge of the construction industry, and several measures have recently been taken to overcome excess CO 2 emission and greenhouse gas emissions associated with cement and concrete production. About 30 billion tons of concrete is consumed annually all over the world. Previously, the production of one ton of concrete generated about 0.5 to 0.6 tons of CO 2 . However, in 2019, the CO 2 generated from concrete production reached 72.5 kg CO 2 /ton. Compared to forty years ago, the quantity of CO 2 generated from concrete production has tripled due to the increase in demand of concrete CR as a partial substitute for fine aggregate were evaluated. Additionally, the mechanical strengths of the SCC blend mixes were also evaluated. Similar research has been conducted on conventional concrete; therefore, it is also adequate to examine these properties in SCC to bridge the research gap.

Materials
For this study, Type 1 Ordinary Portland Cement with a specific gravity of 3.5 obtained in accordance with BS EN 196-6 [19] requirements were used throughout this study. The chemical properties and specific gravity of the cement, fly ash, and CCR are presented in Table 1. Fine aggregate, coarse aggregate, and CR of particle gradation curve combined together as shown in Figure 1 were used. The fine aggregate grading shows a similar particle size with CR and belongs to the zone II class based on the grading limit on [20]. The coarse particle sizes are dominantly 53.77 and 41.49% as specified by EFNARC [21]. A high-range water-reducing admixture was added by weight of cementitious materials to achieve the self-compaction. The dosage of the superplasticizer was used based on the manufacturer's specification of 1.3 to 9.8 mL/kg of cementitious materials. environmentally friendly materials in SCC production. The equivalent CO2 emission and production cost for the SCC mixes containing fly ash and CCR as supplementary cementitious materials, and CR as a partial substitute for fine aggregate were evaluated. Additionally, the mechanical strengths of the SCC blend mixes were also evaluated. Similar research has been conducted on conventional concrete; therefore, it is also adequate to examine these properties in SCC to bridge the research gap.

Materials
For this study, Type 1 Ordinary Portland Cement with a specific gravity of 3.5 obtained in accordance with BS EN 196-6 [19] requirements were used throughout this study. The chemical properties and specific gravity of the cement, fly ash, and CCR are presented in Table 1. Fine aggregate, coarse aggregate, and CR of particle gradation curve combined together as shown in Figure 1 were used. The fine aggregate grading shows a similar particle size with CR and belongs to the zone II class based on the grading limit on [20]. The coarse particle sizes are dominantly 53.77 and 41.49% as specified by EFNARC [21]. A high-range water-reducing admixture was added by weight of cementitious materials to achieve the self-compaction. The dosage of the superplasticizer was used based on the manufacturer's specification of 1.3 to 9.8 mL/kg of cementitious materials.

Mix Proportioning
Percentage replacement was generated around the optimized mix from the existing literature to elaborately predict the effect of the green replacement materials on properties of SCC. Hence, eighteen blends of SCC were produced with variables as follows: in the proportion of 0%, 10%, and 20 CR replacement by volume of fine aggregate, and 40% fly ash volume replacement of cement, and 0%, 5%, and 10% CCR replacement by volume of cementitious materials. The mix proportions are presented in Table 2. The mix IDs are numbered according to the percentage replacement of the material. For example, mix number M10CR40F5C signifies a mix containing 10% by volume replacement of fine aggregate with CR, 40% by volume replacement of cement with fly ash, and 5% addition of CCR to cementitious material.

Sample Preparations and Experimental Methods
The batching, mixing, and sampling of the fresh concrete was carried out in accordance with the guidelines outlined in BS 1881-125 [22]. A rotating pan mixer was utilized for the mixing of the fresh concrete. Before mixing, the cement, fly ash, and CCR were ensured to be completely dried and free from lumps, and the aggregates were in saturated surface dry condition to avoid absorption of the mixing water. The fine aggregate was first poured into the mixer, followed by the cement, fly ash, and CCR. They were then allowed to mix for about 30 s. After that, the coarse aggregate and half of the mixing water were added, and the mixing continued. The superplasticizer was mixed with the other half of the mixing water and was poured gently to the concrete in the mixer. The mixing was continued for about 2 min until a completely homogenous paste was achieved. The mixing was carried out at a room temperature of 20 ± 5 • C and controlled relative humidity. Immediately after mixing, the fresh concrete was casted into the molds. Prior to casting, the molds were cleaned and oiled for ease of demolding. The samples were then air dried for 24 h at room temperature before demolding. After demolding, the samples were fully immersed in clean water for the curing periods prior to testing. The compressive strength test was carried out in accordance with EN 12390-3 [16] using a 1000 kN capacity universal testing machine. One-hundred-millimeter cube samples were prepared and cured for 3, 7, 28, 56, and 90 days prior to testing. For each mix and curing period, triplicate samples were tested, and the average result was reported. The flexural strength test was performed in accordance with the guideline outlined in BS EN 12390-5 [23] using the center point loading method. Prisms of 100 mm × 100 mm × 500 mm were prepared and cured for 3, 7, 28, 56, and 90 days before testing. The samples were tested in triplicate for each mix and each curing period, and the mean value was reported. The splitting tensile strength test was performed following the specifications of BS EN 12390-6 [24], using a 1000 kN UTM. Cylindrical samples of 100 mm diameter and 200 mm height were prepared and cured for 3, 7, 28, 56, and 90 days prior to testing. For each mix and curing period, three samples were tested, and the average value was reported.
The cost of the material used in this study was obtained from the market prices and is shown in Table 3. The total cost for each of the mix was calculated using Equation (1).
where i represents the constituent material number in the mix, n represents the total raw materials in the mix, k i represents the cost of raw material i, and m i represents the quantity of raw material i in kg/m 3 . The equivalent CO 2 emission of the concrete constituent materials from cradle to gate is presented in Table 4. The CO 2 emission for the concrete production include that of the batching and mixing and does not include that of transporting the concrete as it is produced and tested in the laboratory. This implies the overall carbon dioxide emission resulting from production, transportation, and mixing processes. The equivalent CO 2 emission of the mixes from cradle to gate was calculated from the unit emission in Table 4 with the mix designs in Table 2 using Equation (2).
where i is the individual constituent material number in the self-compacting ternary blend mix, n is the overall constituent material in the self-compacting ternary blend mix, M i is the quantity of the constituent material i in kg/m 3 , CO 2,(i − J) is the equivalent CO 2, emission of the constituent material i including material and production, transportation, batching and casting of the concrete in (CO 2 -kg/kg).

Cost Analysis of SCC Mixes
The cost summary used to produce each of the SCC blend mixes is presented in Figure 2. It can be observed that the mixes with fly ash cost less than the control mixes due to the lower cost of fly ash in comparison to cement it replaced in the SCC mixes. On the other hand, the cost of the SCC blend increased slightly with the partial replacement of fine aggregate with CR due to the increased cost of the latter compared to the former, the slight increased cost of the CR results from the processing cost of the waste tires into crumb sizes. However, this could be reduced when the CR production became highly commercialized in large quantities. Nevertheless, incorporation of CR in SCC has several benefits ranging from the increase in flexural strength, toughness, and energy absorption, which in turn enhances its durability and ability to last longer, thereby saving the maintenance cost [16]. This is in line with the study of Samarul H. et al. [29], wherein they agreed that the initial cost of concrete is high but cost of maintenance tends to be low. Additionally, the use of CR in concrete promotes waste utilization and prevents the nuisance caused by the disposal of the non-biodegradable waste tires, which occupies useful land space when disposed or buried and generates toxic gases in the atmosphere when burnt. Similarly, sustainable construction is encouraged through the partial replacement of fine aggregate with CR; hence, nature is preserved through human control from exploiting the natural resources reserve over continuous mining of the natural aggregate. As seen in Figure 2, the addition of CCR to the mix reduced the cost of the mixes but not as much as fly ash did; this is because CCR is a common waste and needs no further processing aside from drying, partial grinding, and sieving to be incorporated in concrete. Aside from the lower cost, CCR is beneficial in several other ways; it enhances early strength development of the concrete mix and dissipates the strength reduction associated with the addition of CR. This is in conformity with the research outcome of van der Spek et al. [30].

Cost Analysis of SCC Mixes
The cost summary used to produce each of the SCC blend mixes is presented in Figure 2. It can be observed that the mixes with fly ash cost less than the control mixes due to the lower cost of fly ash in comparison to cement it replaced in the SCC mixes. On the other hand, the cost of the SCC blend increased slightly with the partial replacement of fine aggregate with CR due to the increased cost of the latter compared to the former, the slight increased cost of the CR results from the processing cost of the waste tires into crumb sizes. However, this could be reduced when the CR production became highly commercialized in large quantities. Nevertheless, incorporation of CR in SCC has several benefits ranging from the increase in flexural strength, toughness, and energy absorption, which in turn enhances its durability and ability to last longer, thereby saving the maintenance cost [16]. This is in line with the study of Samarul H. et al. [29], wherein they agreed that the initial cost of concrete is high but cost of maintenance tends to be low. Additionally, the use of CR in concrete promotes waste utilization and prevents the nuisance caused by the disposal of the non-biodegradable waste tires, which occupies useful land space when disposed or buried and generates toxic gases in the atmosphere when burnt. Similarly, sustainable construction is encouraged through the partial replacement of fine aggregate with CR; hence, nature is preserved through human control from exploiting the natural resources reserve over continuous mining of the natural aggregate. As seen in Figure 2, the addition of CCR to the mix reduced the cost of the mixes but not as much as fly ash did; this is because CCR is a common waste and needs no further processing aside from drying, partial grinding, and sieving to be incorporated in concrete. Aside from the lower cost, CCR is beneficial in several other ways; it enhances early strength development of the concrete mix and dissipates the strength reduction associated with the addition of CR. This is in conformity with the research outcome of van der Spek et al. [30]. M0CR40F0C

Equivalent CO 2 Gas Emission of SCC Mixes
The summary of the CO 2 emission from cradle to gate in all the SCC blend mixes is shown in Figure 3. All the mixes have lower CO 2 emissions when compared to the control mix; this is because of the high CO 2 emitted in concrete production, unlike fly ash, which requires zero CO 2 emission except for the minimal CO 2 generated during grinding and transportation of the fly ash [8]. Partial replacement of fine aggregate with CR also increased the CO 2 emission of the mix; this is because of the higher CO 2 emission in CR compared to natural aggregate, as could be seen in Table 4. As for CR, the high CO 2 emission emanates from the grinding of the waste tire to smaller sizes and transportation; thus, CR alone contains no CO 2 . More so, the addition of CCR decreases the CO 2 emission but not as much as fly ash because of the greenhouse gas generated during acetylene gas production that generates calcium carbide residue as a byproduct. This is in line with the research outcome of Fennell et al. [31]. Therefore, more sustainable and green SCC mixes can be obtained by reducing and replacing the amount of cement with supplementary cementitious materials such as fly ash and CCR. These materials, when used in high percentages to replace cement, result in a decrease in strength development, yet they decrease the CO 2 emission of the SCC and also reduce the cost of producing the mix.

Equivalent CO2 Gas Emission of SCC Mixes
The summary of the CO2 emission from cradle to gate in all the SCC blend mixes is shown in Figure 3. All the mixes have lower CO2 emissions when compared to the control mix; this is because of the high CO2 emitted in concrete production, unlike fly ash, which requires zero CO2 emission except for the minimal CO2 generated during grinding and transportation of the fly ash [8]. Partial replacement of fine aggregate with CR also increased the CO2 emission of the mix; this is because of the higher CO2 emission in CR compared to natural aggregate, as could be seen in Table 4. As for CR, the high CO2 emission emanates from the grinding of the waste tire to smaller sizes and transportation; thus, CR alone contains no CO2. More so, the addition of CCR decreases the CO2 emission but not as much as fly ash because of the greenhouse gas generated during acetylene gas production that generates calcium carbide residue as a byproduct. This is in line with the research outcome of Fennell et al. [31]. Therefore, more sustainable and green SCC mixes can be obtained by reducing and replacing the amount of cement with supplementary cementitious materials such as fly ash and CCR. These materials, when used in high percentages to replace cement, result in a decrease in strength development, yet they decrease the CO2 emission of the SCC and also reduce the cost of producing the mix.

Compressive Strength of SCC Mixes
The compressive strength results for selected SCC blends without and with fly ash are presented in Figure 4 and Figure 5, respectively. The compressive strength of the mixes generally increased with curing age and decreased with the addition of the optimum 40% fly ash content to the mix. The increase in strength with the age of curing is due to the hydration of cement and the pozzolanic reaction of fly ash. It is also a result of modification of the bonding properties of the binders' hydrates [32]. The 28-day compressive strength of the SCC mix without fly ash ranged from 38 to 45 N/mm 2 but decreased to the range of 36 to 40 N/mm 2 on replacement of 10% fine aggregate with CR and further decreased to the range of 32

Compressive Strength of SCC Mixes
The compressive strength results for selected SCC blends without and with fly ash are presented in Figures 4 and 5, respectively. The compressive strength of the mixes generally increased with curing age and decreased with the addition of the optimum 40% fly ash content to the mix. The increase in strength with the age of curing is due to the hydration of cement and the pozzolanic reaction of fly ash. It is also a result of modification of the bonding properties of the binders' hydrates [32]. The 28-day compressive strength of the SCC mix without fly ash ranged from 38 to 45 N/mm 2 but decreased to the range of 36 to 40 N/mm 2 on replacement of 10% fine aggregate with CR and further decreased to the range of 32.3 to 35.4 N/mm 2 on 20% fine aggregate replacement with CR. The maximum 45 N/mm 2 value was obtained on replacement of 5% of the cementitious materials with CCR, which was an 8.4% increase in the strength of the control mix. The same trend was maintained by the mixes containing fly ash. The decrease in strength with CR incorporation can be attributed to the poor bonding between the rubber particles and cement paste, resulting in premature failure with load application and consequently a reduction in strength. Additionally, CR, due to its hydrophobic nature, entraps air during mixing; after the concrete has dried up, this entrapped air created pores in the hardened cement matrix. The pores generate weak paths for which premature failure occurs with load application [16,33,34]. Another reason is due to the increased thickness of the interfacial transition zone between the hardened concrete paste matrix and CR particles, resulting in a low bond between them and forms micro-cracks which consequently cause premature failure. This is in line with the finding of Mohammed and Adamu [33]. Therefore, moderate proportions of CCR and fly enhance the compressive strength of SCC. The pozzolanic reaction between Ca(OH) 2 from cement hydration products and CCR with the SiO 2 from fly ash reacts to produce more C-S-H gels, a vital compound that enhances strength development in concrete [35]. Moreover, the incorporation of a higher proportion of CCR and fly ash results in increased water demand or superplasticizer for consistency because its larger surface area and the mix has low water content, which causes agglomeration of the particles and poor consistency of the SCC mix and consequently leads to reduced compressive strength [36]. load application [16,33,34]. Another reason is due to the increased thickness of the interfacial transition zone between the hardened concrete paste matrix and CR particles, resulting in a low bond between them and forms micro-cracks which consequently cause premature failure. This is in line with the finding of Mohammed and Adamu [33]. Therefore, moderate proportions of CCR and fly enhance the compressive strength of SCC. The pozzolanic reaction between Ca(OH) from cement hydration products and CCR with the SiO2 from fly ash reacts to produce more C-S-H gels, a vital compound that enhances strength development in concrete [35]. Moreover, the incorporation of a higher proportion of CCR and fly ash results in increased water demand or superplasticizer for consistency because its larger surface area and the mix has low water content, which causes agglomeration of the particles and poor consistency of the SCC mix and consequently leads to reduced compressive strength [36].
From Figure 4, it can be observed that mixes containing CCR such as M0CR5C and M0CR10C demonstrated higher early strength development at 3 days compared to mixes without CCR such as M0CR0C. This can be attributed to the higher CaO (cementitious element) content of CCR, which is a major compound also found in cement, reacting during the early hydration process to produce the compound for strength development in the concrete. As CCR is a highly reactive pozzolanica material, the pozzolanic reaction occurs at earlier ages, thereby enhancing the early strength development  From Figure 4, it can be observed that mixes containing CCR such as M0CR5C and M0CR10C demonstrated higher early strength development at 3 days compared to mixes without CCR such as M0CR0C. This can be attributed to the higher CaO (cementitious element) content of CCR, which is a major compound also found in cement, reacting during the early hydration process to produce the compound for strength development in the concrete. As CCR is a highly reactive pozzolanica material, the pozzolanic reaction occurs at earlier ages, thereby enhancing the early strength development

Splitting Tensile Strength of SCC Mixes
The results of the splitting tensile strength of various SCC mixes without and w optimum 40% fly ash is presented in Figures 6 and 7. The splitting tensile strength of the mixes increased with curing age and decreased on adding the optimum 40% fly a content to the mix. The 28 days splitting tensile strength of the SCC mix without ranged from 2.9 to 4.1 N/mm 2 but decreased to the range of 2.1 to 3.6 N/mm 2 on repla ment of 40% of cement with fly ash. Generally, increment in splitting tensile strength w observed on incorporating CR and CCR into the mix but decreased beyond 10% CR a 5% CCR, though not below that of the control mix. Hence, mix M10CR5C a M10CR40F5C had the maximum splitting tensile strength value for without and with ash mixes, respectively. The increase in the splitting tensile strength of concrete result from the increased micro fiber nature of CR, which bridges the cracks in the concre thereby reducing the chance of total failure [33]. However, the decrease in the splitti tensile strength when the proportion of CR is further increased is based on the weak bon ing between harden concrete paste matrix and rubber particles, which results in sm cracks and consequently sudden strength loss [37]. The presence of CCR enhanced t splitting tensile strength. For example, the splitting tensile strength of mix M10CR0C co taining 10% CR and 0% CCR was increased by 2.4% on incorporation of 5% CCR on m M10CR5C. This increment is caused by a large surface area and the irregular morpholo of CCR particles which enhanced the bond between the hardened cement paste and a gregates [38]. This is similar to the finding of Bayuaji et al. [39].

Splitting Tensile Strength of SCC Mixes
The results of the splitting tensile strength of various SCC mixes without and with optimum 40% fly ash is presented in Figures 6 and 7. The splitting tensile strength of all the mixes increased with curing age and decreased on adding the optimum 40% fly ash content to the mix. The 28 days splitting tensile strength of the SCC mix without FA ranged from 2.9 to 4.1 N/mm 2 but decreased to the range of 2.1 to 3.6 N/mm 2 on replacement of 40% of cement with fly ash. Generally, increment in splitting tensile strength was observed on incorporating CR and CCR into the mix but decreased beyond 10% CR and 5% CCR, though not below that of the control mix. Hence, mix M10CR5C and M10CR40F5C had the maximum splitting tensile strength value for without and with fly ash mixes, respectively. The increase in the splitting tensile strength of concrete resulted from the increased micro fiber nature of CR, which bridges the cracks in the concrete, thereby reducing the chance of total failure [33]. However, the decrease in the splitting tensile strength when the proportion of CR is further increased is based on the weak bonding between harden concrete paste matrix and rubber particles, which results in small cracks and consequently sudden strength loss [37]. The presence of CCR enhanced the splitting tensile strength. For example, the splitting tensile strength of mix M10CR0C containing 10% CR and 0% CCR was increased by 2.4% on incorporation of 5% CCR on mix M10CR5C. This increment is caused by a large surface area and the irregular morphology of CCR particles which enhanced the bond between the hardened cement paste and aggregates [38]. This is similar to the finding of Bayuaji et al. [39]. Sustainability 2022, 14, x FOR PEER REVIEW 10 of 14

Flexural Strength of SCC Mixes
The results of flexural strength of various SCC blends without and with optimum 40% fly ash are presented in Figure 8 and Figure 9, respectively. The highest 28-day flexural strength of 6.7 MPa without fly ash was achieved with mix M0CR5C in proportions of 0% and 5% of CR and CCR, respectively. Mix M20CR0C has the lowest flexural strength of 4.9 MPa with a mixed proportion of CR and CCR at 20% and 0%, respectively. The increase in flexural strength associated with the incorporation of CCR was due to the increased pozzolanic reaction resulting from the strengthening of the interfacial zone between CR-cement paste and aggregate. The average flexural strength of SCC ranges from 3 to 6 MPa; as such, the flexural strength of all the mixes falls within this range with the

Flexural Strength of SCC Mixes
The results of flexural strength of various SCC blends without and with optimum 40% fly ash are presented in Figure 8 and Figure 9, respectively. The highest 28-day flexural strength of 6.7 MPa without fly ash was achieved with mix M0CR5C in proportions of 0% and 5% of CR and CCR, respectively. Mix M20CR0C has the lowest flexural strength of 4.9 MPa with a mixed proportion of CR and CCR at 20% and 0%, respectively. The increase in flexural strength associated with the incorporation of CCR was due to the increased pozzolanic reaction resulting from the strengthening of the interfacial zone between CR-cement paste and aggregate. The average flexural strength of SCC ranges from 3 to 6 MPa; as such, the flexural strength of all the mixes falls within this range with the

Flexural Strength of SCC Mixes
The results of flexural strength of various SCC blends without and with optimum 40% fly ash are presented in Figures 8 and 9, respectively. The highest 28-day flexural strength of 6.7 MPa without fly ash was achieved with mix M0CR5C in proportions of 0% and 5% of CR and CCR, respectively. Mix M20CR0C has the lowest flexural strength of 4.9 MPa with a mixed proportion of CR and CCR at 20% and 0%, respectively. The increase in flexural strength associated with the incorporation of CCR was due to the increased pozzolanic reaction resulting from the strengthening of the interfacial zone between CR-cement paste and aggregate. The average flexural strength of SCC ranges from 3 to 6 MPa; as such, the flexural strength of all the mixes falls within this range with the maximum exceeding it. This implies that partial replacement of cementitious materials with CCR in the right proportion will result in an SCC of quality flexural strength. The results of the mix containing fly ash in Figure 9 followed the same trend. Overall, this is in line with the result obtained from the research conducted by Ganesan et al. [40]. The increse in flexural strength due to CR addition can be attributed to the higher flexibility, bending ability and fibrous nature of the CR in comparison to fine aggregate it partially replaced. This resulted to an improvement in post-cracking bending resistance, giving the SCC some capability of resisting some bending loading, even after failure [33]. maximum exceeding it. This implies that partial replacement of cementitious materials with CCR in the right proportion will result in an SCC of quality flexural strength. The results of the mix containing fly ash in Figure 9 followed the same trend. Overall, this is in line with the result obtained from the research conducted by Ganesan et al. [40]. The increse in flexural strength due to CR addition can be attributed to the higher flexibility, bending ability and fibrous nature of the CR in comparison to fine aggregate it partially replaced. This resulted to an improvement in post-cracking bending resistance, giving the SCC some capability of resisting some bending loading, even after failure [33].  maximum exceeding it. This implies that partial replacement of cementitious materials with CCR in the right proportion will result in an SCC of quality flexural strength. The results of the mix containing fly ash in Figure 9 followed the same trend. Overall, this is in line with the result obtained from the research conducted by Ganesan et al. [40]. The increse in flexural strength due to CR addition can be attributed to the higher flexibility, bending ability and fibrous nature of the CR in comparison to fine aggregate it partially replaced. This resulted to an improvement in post-cracking bending resistance, giving the SCC some capability of resisting some bending loading, even after failure [33].

Conclusions
In this study, SCC mixes were produced, where two series of mixes were prepared. In this series, 100% OPC was used, and CR was used as a partial replacement by volume of fine aggregates, and CCR was used as a partial replacement by volume of cementitious materials. In the second series, 40% cement was replaced with fly ash, CR was used as a partial replacement to fine aggregate, and CCR was used as a partial replacement to cementitious materials. Based on the experimental work and results analysis, the following conclusions were drawn: 1.
Fly ash utilization in SCC as SCM significantly reduced the cost of production of the concrete, wherein up to 14% reduction in cost was achieved with replacing 40% cement using fly ash. However, CR increased the initial cost of the green self-compacting concrete ternary blend by 2% when compared to the control mix, and these continued to reduce at greater percentage replacements.

2.
Fly ash and CCR were effective in reducing the greenhouse CO 2 emission of SCC during production, wherein up to a 35% reduction was achieved with the replacement of 40% cement using fly ash and 4% reduction with replacing 5% cement with CCR. On the contrary, replacement of fine aggregate with CR has a significantly less negative effect on the CO 2 emission of the SCC, wherein 10% CR as a replacement to fine aggregate increased the CO 2 emission by less than 1%. 3.
The use of fly ash as SCM and CR as a partial replacement to fine aggregate contributed negatively to its compressive strength, flexural strength, and splitting tensile strength of the SCC. 4.
The addition of CCR to the SCC mixes improved its mechanical strengths and partially mitigated the negative effects of fly ash and CR on the concrete's strengths. The addition of CCR increased precipitation of the hydration products from cement and fly ash and contributed to the early-age strength development.

5.
Therefore, fly ash and CCR are recommended for the production of green, sustainable, environmentally friendly, and cost-effective SCC with lower CO 2 emissions and less cost, which will be particularly beneficial now that the world is facing the challenges of global warming.